© 2012 Rodriguez-Castellon et al., licensee InTech. This is an open access chapter distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Transition Metal Sulfide Catalysts for Petroleum Upgrading – Hydrodesulfurization Reactions
A. Infantes-Molina, A. Romero-Pérez, D. Eliche-Quesada, J. Mérida-Robles, A. Jiménez-López and E. Rodríguez- Castellón
Additional information is available at the end of the chapter
Environmental catalysis researchers worldwide have focused much attention on the development of catalytic systems capable of reducing the sulfur amount present in petroleum feedstocks until levels globally established by the recently enacted environmental protection laws. In this regard, the maximum sulfur content present in diesel fuel to obtain an Ultra Low Sulfur Diesel (ULSD) is of 10 ppm in the European Union from the beginning of 2009 with the entry into force of the Euro V fuel standard directive. Meanwhile this limit is slightly higher in the United States, 15 ppm, regulated by the Environmental Protection Agency (EPA) (Hsu & Robinson, 2006). Thus, the development of highly active and selective HDS catalysts, capable of processing these feeds, is one of the most important problems that the petroleum industry has to face nowadays.
Transition metal sulfides (TMS) have been traditionally used as active phases in hydrotreating catalysts since they are known to be efficient systems for catalyzing hydrotreating reactions. Concretely cobalt or nickel promoted molybdenum–tungsten sulfides are well established as the active species for commercial hydrodesulfuration (HDS) catalysts and mainly porous-alumina as a support. Amelioration has been achieved by modifying the properties of these sulfide systems, although the nature of the active phase has hardly been modified during many decades (Song & Ma, 2003). One direction for current research focuses on the use of new types of supports. Studies on nickel sulfided catalysts have concluded that supports, such as Al2O3, strongly interact with Ni2+ ions avoiding their sulfidation (Gil et al., 1994). Ni2+-alumina interactions may be weakened by using carriers such as alumina-pillared compounds, where the aluminium oxide is diluted within a layered inorganic matrix inducing a permanent porosity. These materials have been used as catalysts supports in hydrotreating reaction, showing interesting results (Kloprogge
et al., 1993; Occelli & Rennard, 1988). On the other hand, mesoporous silica sieves have become a real alternative to alumina due to their hexagonal array of uniform mesopores and a very high surface area, presenting potential catalytic application for reactions involving bulky molecules, including hydrodesulfurization of petroleum fractions (Corma et al., 1995; Song & Reddy, 1999). In the same way, HMS type materials have been widely studied in this type of reactions (Nava et al., 2011; Zepeda et al., 2005). The intercalation of heteroatoms such as Al, Ti, Ga or Zr into the silica framework not only improves the material stability but also generates new acid, basic or redox functions that extend their application in new fields of catalysis. Thus, zirconium doped mesoporous silica with high surface area, mild acidity and high stability (Rodríguez-Castellón et al., 2003) have shown interesting properties as a support for catalytic fuel processing in reactions such as the hydrogenation, hydrogenolysis and hydrocracking of tetralin (Eliche-Quesada et al., 2003a, 2003b, 2004, 2005). The use of SBA-15 as a support for hydrotreating catalysts has presented several advantages with regard to HMS and MCM-41 mesoporous solids, since SBA-15 material has thicker pore walls and better hydrothermal stability, which are very important properties in hydrotreating processes due to the severe reaction conditions employed (Vradman et al., 2003). Recently, Gómez Cazalilla et al. (Gómez-Cazalilla et al., 2007) have proposed a cheap sol-gel synthesis route for SBA-15 and aluminium doped SBA-15, with sodium silicate as the silica source. The resulting materials have shown interesting properties as catalyst supports in hydrotretating reactions (Gómez-Cazallila et al., 2009a, 2009,b).
Other direction for current research focuses on the use of new active phases for developing high-performance HDS catalysts. The pioneering work of Pecoraro and Chianelli (Pecoraro & Chianelli, 1981) reported the great catalytic activity of bulk transition metals sulfides (TMS). Such metals were plotted into a curve called “volcano plot” where the HDS activity per mole of metal versus the M-S bond strength was plotted, the RuS2 phase being the most active (Toulhoat et al., 1999). Nonetheless when the RuS2 phase is supported, the results found in literature are diverse. On one hand a lower activity was observed due to its reduction into metallic ruthenium under the reducing conditions employed in the catalytic test (De los Reyes, et al., 1990) and if it is supported on alumina, sulfiding temperatures higher than 773 K are required to form the RuS2 phase with pyrite-like structure, which is the true active phase for hydrotreating reactions. Nonetheless, it has been reported that Ru/γ-Al2O3 catalyst sulfided in 100% H2S at 673 K possessed about 7-fold higher thiophene conversion rates than CoMo/γ-Al2O3 when the surface of the active area is considered (Kuo et al., 1988).
Quartararo et al. (Quartararo et al., 2000) perfectly describe that there are many factors during the synthesis of ruthenium sulfide catalysts that must be taken into account for controlling their physicochemical properties, and as a consequence for achieving a good performance with this kind of catalysts. It is recommended no calcination after the incorporation of ruthenium chloride, while the sulfiding mixture should be H2S/N2 to achieve a high degree of sulfurization and avoid the reduction of the RuS2 phase formed (De los Reyes, 2007). Furthermore, the sulfiding temperature influences the catalytic behaviour (De los Reyes et al., 1991) as well as the crystallographic orientations that induce the
Transition Metal Sulfide Catalysts for Petroleum Upgrading – Hydrodesulfurization Reactions
preference toward HDS and hydrogenation (HYD) reactions. One of the main goals to reach is the stabilization of such a phase under the reaction conditions. Ishihara et al. (Ishihara et al., 1992) were the first to report the addition of alkali metals to RuS2 catalysts supported on Al2O3. The addition of NaOH did not improve the HDS reaction because of the poisoning of some sites. Nonetheless, a cesium-promoted Ru catalyst with Ru/Cs molar ratio of 1:2 exhibited HDS activities comparable to that of conventional Co-Mo catalyst (Ishihara et al., 2003). The insertion of atoms like cesium seems to enhance the number of labile sulfur atoms, aids to stabilize the RuS2 active phase as it strengths Ru-S bond of ruthenium sulfide, promotes the C-S bond scission of dibenzothiophene (DBT) and therefore the catalytic activity increases (Ishihara et al. 2004). However, if a Cs excess is present, the formation of H2S and regeneration of coordinatively unsaturated sites are prevented, which results in a decrease in the catalytic activity.
With these premises, catalysts for HDS reaction based on molybdenum, tungsten and ruthenium sulfide are described. The role of promoters and material supports on the catalytic activity are reviewed. In this regard, the support effect on HDS activity on molybdenum and tungsten sulfided catalysts promoted with nickel and cobalt are evaluated by using fluorinated alumina α-zirconium phosphate materials, zirconium doped mesoporous silica (Zr-MCM) and a commercial -Al2O3. Moreover the HDS activity of alternative phases such as RuS2 is also described considering not only the role of the support (MCM-41, Zr-MCM-41, -Al2O3, SBA-15, Zr-SBA-15 and Al-SBA-15) employed but also the addition of a stabilizing agent such as Cs and the cesium precursor salt employed. The catalysts were characterized by X-ray diffraction (XRD), N2 adsorption–desorption isotherms at 77 K, NH3-temperature-programmed desorption (NH3-TPD), X-ray photoelectron spectroscopy (XPS), H2-temperature-programmed reduction (H2-TPRS), transmission electron microscopy (TEM) and DRIFT spectra of adsorbed NO.
2. Tungsten and Molybdenum sulfide catalysts
2.1. HDS of Thiophene
Nickel, molybdenum and nickel-molybdenum sulfided catalysts supported on alumina- pillared -zirconium phosphate ZrAl3.39O1.12(OH)1.60F4.90 H0.57(PO4)2 (Mérida et al., 1996), with different loadings of Ni and Mo are described. The catalysts were tested in the thiophene HDS reaction at 673 K, using an automatic microcatalytic flow reactor under atmospheric pressure. A hydrogen flow of 50 cm3 min-1 containing 4.0 mol% thiophene was fed to the reactor. Monometallic nickel catalysts were prepared following the incipient wetness method with ethyl alcohol solutions of nickel(II) nitrate (Ni(NO3)2) and nickel metallic loadings of 4, 8 and 12 wt%, denoted as 4wt%Ni, 8wt%Ni and 12wt%Ni, respectively. A catalyst only containing molybdenum (13wt%Mo), was also synthesized with aqueous solution of ammonium molybdate (NH4)6Mo7O244H2O. Finally, another set of catalysts containing both nickel and molibdenum were prepared by successive
Click here to load reader